Table of Contents

Tests frequency and Acceptance Criteria in Testing of material for structures as per quality assurance level Q-4 of IRC: SP47-1998 and other IRC, and MORTHย Specifications.

S. No | Type of Construction | Frequency | Location | Acceptance Criteria | ||

1.0 ย ## Frequency and Acceptance Criteria in Testing:1.1 ## For Coarse Aggregate: | ||||||

(i) | Moisture Content (IS:383, IS:2386 Part III) | Daily/at every day ofย concreting | Plant | Max. 5% | ||

(iI) | Specific Gravity (IS:383, IS:2386 – Part III) | 1) One per source and when source changes | Plant | – | ||

(iii) | Gradation/Sieve Analysis (IS:383, IS:2386 โ Part 1) | Daily | Plant | Table 1000-1 of MOSRTH Specifications for Road and Bridge Works | ||

(iv) | Aggregate Impact Value/Los Angles Abrasion Value (IS:383, IS:2386 Part IV) | 1) One per source ย 2)ย Weekly | Plant | Aggregate Impact Value 45% Max. for concrete other than for wearing surfaces; 30% Max. for concrete for wearing surfaces. ย Los Angles Abrasion value 50% Max. for Concrete other than for wearing surfaces; 30% Max. for Concrete for wearing surfaces. | ||

(vi) | Flakiness Index (IS:383,IS:2386 Part 1) | 1) One per source ย 2) Weekly | Plant | Max.ย 35% ย MORTH Clause of 1007. | ||

(vii) | Water absorption of Aggregate (IS383, IS:2386 Part III) | 1)One per source ย 2) when sourcing changes | Plant | Max.ย ย 10% | ||

(viii) | Soundness (Magnesium and sodium sulphate) ย IS:383, IS:2386 Part V) | 1) One per source | Plant | Sodium sulphate ย Max.ย 12% Magnesium sulphate Max.ย 18% | ||

(ix) | Alkali-Aggregate reactivity (IS:383, IS:2386 Part VII, IS: SP-23) | 1) One per source | Plant | Fig. 6 of IS:2386 Part VII | ||

(x) | Petrographic Analysis (IS:383, ASTM 295, IS:2386 Part VIII) | 1)ย ย ย One per source | Plant | As per IS: 2386 Part VIII | ||

1.2## For Fine Aggregate: | ||||||

(i) | Silt Content (IS:383, IS2386 Part II) | Daily | Plant | Max. 3% | ||

(ii) | Moisture Content (IS:383,IS:2386) | At every day of concreting | Plant | Max. 5% | ||

(iii) | Gradation/Sieve Analysis, Fineness Modulus (IS:383, IS:2386 โPart III) | Daily | Plant | Table 1000-2 of MORTH Specifications for Road and Bridge Works. ย Fineness Modulus Min. 2.0% Max 3.5% | ||

(iv) | Water absorption of Aggregate (IS:383, IS:2386 Part 3) | 1) One per source ย 2)when sourcing changes | Plant | Max 10% | ||

(ix) | Soundness (Magnesium and Sodium Sulphate) ย IS:383, IS:2386 Part V) | One per source | Plant | Sodium sulphate Max. 10% ย Magnesium sulphate Max. 15% | ||

1.3## For Ordinary Portland Cement: | ||||||

1.3.1 |
| ย | ย | ย | ||

(i) | Initial Setting Time | 1) One per supply ย 1) Monthly | Plant | Min. 30 minutes | ||

(ii) | Final Setting Time | 1) One per supply ย 2) Monthly | Plant | ย Max. 600 minutes | ||

(iii) | Soundness (by Le-Chatlierโs method) ย By Autoclave (%) (IS:4031) | One per supply | Plant | Max. 10mm ย Max. 0.8% | ||

(iv) | Fineness (by Blaineโs air permeability method) IS:4031 part-2 | One per supply | Plant | Min. 225 m^{2}/kg | ||

(v) | Compressive strength | 1) One per supply ย 2) Monthly | Plant | Min. 23 MPa (3 days) ย Min. 33 MPa (7 days) Min. 43 MPa (28 days) | ||

1.3.2 | ## Chemical Tests (IS:8112) | ย | ย | ย | ||

(i) | Loss on Ignition | One per supply | Plant | Max. 5% | ||

(ii) | Insoluble residue | One per supply | Plant | Max. 2% | ||

(iii) | Alumina Iron Oxide ratio | One per supply | Plant | Min. 0.66 | ||

(iv) | Lime Saturation factor | One per supply | Plant | Min. 0.66 Max. 1.02 | ||

(v) | Magnesia | One per supply | Plant | Max. 6% | ||

(vi) | Sulphuric anhydride | One per supply | Plant | Max. 3% | ||

(vii) | Alkalies | One per supply | Plant | Max. 0.6% | ||

(viii) | Chlorides | One per supply | Plant | Max. 0.05% | ||

1.4 ## For Water (IRC:21-2000/IS:3025): | ||||||

(a) | The volume of 0.02N NaOH required to neutralize 100 ml sample of water using phenolphthalein as an indicator (IS:3025) | 1) One per supply ย 2) Monthly | In situ | Max. 5.0ml | ||

(b) | The volume of 0.02Nย H_{2}SO_{4ย ย }ย requiredย to neutralize 100 ml sample of water using methyl orange as an indicator (IS:3025) | 1) One per source ย 2) Thrice in a year | Insitu | Max. 25.0ml | ||

(c) | Solids (IS:456, IS:3025) | ย | ย | ย | ||

(i) | Organic | 1) One per source ย 2) Thrice in a year | Insitu | 200 mg/lit | ||

(ii) | Inorganic | 1) One per source ย 2) Thrice In a year | Insitu | 3000 mg/lit | ||

(iii) | Sulphates (SO_{4}) | 1) One per source ย 2) Thrice in a year | Insitu | 500 mg/lit | ||

(iv) | Chlorides (CI) | 1) One per source ย 2) Thrice in a year | Insitu | 500 mg/lit | ||

(v) | Suspended matter | 1) One per source ย 2) Thrice in a year | Insitu | 2000 mg/lit | ||

(d) | pH | 1) One per source ย 2) Thrice in a year | Insitu | Min. 6.0 | ||

1.5## Acceptance Criteria in Testing For Admixture: | ||||||

(i) | Chloride Content (IS:9103, IS:6925) | 1) One per supply ย 2) Yearly | Plant | Within 10% of the value or within 0.2% whichever is greater as stated by the manufacturer. | ||

(ii) | Dry Material content (IS:9103) | 1) One per supply ย 2) Yearly | Plant | 5% of liquid admixtures respectively of the value state by the manufacturer | ||

(iii) | Ash content (IS:9103) | 1) One per supply ย 2) Yearly | Plant | Toย be within 5% of the value stated by the manufacturer | ||

(iv) | Relative density (IS:9103) | 1) One per supply ย 2) Yearly | Plant | To be within 2% of the value stated by the manufacturer. | ||

1.6## Acceptance Criteria in Testing for Concrete: | ||||||

(i) | Chloride Content (IS:10262, IS:456,IRC:21) | ย Oneย per New source | Plant | Max. 0.1% by mass of cement for PSC and 0.3% for RCC | ||

(ii) | Sulphate Content as SO_{3ย }(IS:456, IRC:21) | Oneย per New source | Plant | Max. 4% by mass of cement | ||

(iii) | Air Content (Table 3, IS:10262) | Monthly | Plant | Nominal max. size of aggregate | Entrapped air as % of the volume of concrete | |

10mm | 3.0 | |||||

20mm | 2.0 | |||||

40mm | 1.0 | |||||

(iv) | Mix proportion | Every batch of concrete | Plant | As per approved mix design | ||

(v) | Sample of the cube (A sample means a set of 3 cubes) | Every concrete spread over the entire period of concreting | Insitu | Qty of concrete (m3) | No. of samples | |

<30 ย 31-50 51 & above | 3 ย 4 4 + One additional for each 50 m3 | |||||

(vi) | Workability (Slump) (IS:10262,IS:456, IRC:21) | Every batch of concrete at despatch as well as the delivery point | In situ | As specified for specific Grade, structural component and method of concreting | ||

(vii) | Temp. of Fresh concrete (MORTH Specs. Clause 1709) | Every batch of concrete at despatch as well as the delivery point | Insitu | Min. 5ยฐ C ย Max. 40ยฐC | ||

(viii) | The density of Hardened Concrete | Every batch of concrete | Plant | – | ||

(ix) | Permeability (MORTH Specs. Clause 1716.5) | As and when required | Plant | Depth of penetration of water Max. 25mm | ||

(x) | Cube Strength of Concrete | Every batch of concrete | Plant | (i)ย Mean strength from any group of four consecutive samples should be greater than Characteristic strength + 3 MPa ย (ii)ย Individual sample not less thanย Characteristic str โ 3 MPa | ||

1.7## Acceptance Criteria in Testing For Mastic Asphalt: | ||||||

(a) | Binder | Oneย sampleย per Lot | Stacking yard | As per Table 500-29 of MORT&H Specifications for Road and Bridge Works | ||

(b) | Filler (Limestone powder) (IS:1514) | Oneย sampleย per Lot | Stacking yard | Powder passing the 0.075 mm sieve and having calcium carbonate content not less than 80% by weight. | ||

(c) | Mix proportions | One sample per Lot | Insitu | As per JMF to be laid between 175ยฐ and 210ยฐC | ||

d) | Hardness no IS:1195-1978 | In situ | In situ | 60-80 at 25ยบC before addition of C.A. and 10-20 at 25ยบC at the time of after addition of C.A. |